Journal of Physical Science and Application 7 (2) (2017) 18-26 doi: 10.17265/2159-5348/2017.02.003 D DAVID PUBLISHING
Carlo Cristalli, Pietro Agostini, Davide Bernardi, Nicola Bettocchi, Luigi Masotti and Sandro Storai ENEA CR Brasimone, Camugnano (BO) 40032, Italy
Abstract: Creep-fatigue is a damage mechanism where cyclic deformation damage (fatigue) is enhanced by creep damage and vice versa. Factors affecting the creep-fatigue damage are stress level (or, equivalently, strain range), temperature, hold time period, material softening/hardening and number of cycles. Moreover, environmental effects can accelerate the creep-fatigue interaction (oxidation, hot corrosion, irradiation, etc.). The activity described in this paper was planned to perform tests on 9Cr-1Mo ferritic/martensitic steel (P91) combining fatigue cycles and constant tensile and compressive holding periods. A preliminary basic fatigue characterization campaign in the LCF (low cycle fatigue) regime was carried out by performing a series of strain controlled tests, each at the same temperature (550 °C), using two different values for the total strain range (1% and 0.6%) and the same total strain rate (2×10-3 s-1). The tests were carried out with a strain ratio of –1, i.e., in fully reversed cyclic conditions. In this paper we illustrate the results obtained by testing in air P91 (9Cr-1Mo) ferritic/martensitic steel, introducing different dwell periods (either in strain or load control) and observing how these affect the fatigue life of the specimens. The final aim of the activity is to investigate how much detrimental is the effect of the holding periods on the fatigue life in order to validate the creep-fatigue interaction diagram presently adopted in RCC-MRx code for the P91 steel.
Key words: P91, creep-fatigue, fatigue damage, creep damage, interaction diagram, RCC-MRx, softening.
1. Introduction condition; Nf(fatigue)= Number of cycle to failure in LCF conditions; tH: hold time (hrs); tR: creep rupture Modified 9Cr-1Mo steel is a candidate steel for use time (hrs); D: failure criterion. The failure criterion in steam generators of nuclear power plants, to varies in agreement with the adopted standards. achieve a design life of 60 years and operational Criterion D is described by a curve in a “fatigue temperature 550 °C. To ensure the longevity and safe damage—creep damage” plot. A curve that bilinearly operation of a nuclear power plant, it is essential to connects (1, 0); (0.3, 0.3) and (0, 1) coordinates is prevent creep-fatigue damage and evaluate long-term employed in the RCC-MRx code  while the bilinear creep-fatigue life. The linear damage rule is the most correlation between (1, 0); (0.1, 0.01) and (0, 1) well-known method that is typically used to evaluate coordinates is adopted in the ASME code  (Fig. 1). creep-fatigue life. When the linear sum of fatigue One of the objectives of the present work is to clarify damage and creep damage of a material reaches a the discrepancy between the two curves of damage critical value, the material fails. Creep damage is limit. The first and second items in the left side of Eq. typically calculated using time fraction rule or (1) are fatigue damage and creep damage, respectively. ductility exhaustion approach. The following Eq. (1) The time fraction rule requires a creep rupture curve  is used to evaluate creep-fatigue life by the time to evaluate creep damage. In ASME III NH , JSME fraction rule:  and RCC-MRx  the calculation procedure of (1) creep damage utilizes the time-fraction approach, where, N = Number of cycle to failure in the tested while BS-R5  is currently the only code following a
“ductility exhaustion” methodology. Corresponding author: Carlo Cristalli, research field: mechanical characterization of nuclear materials.
Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91 19
Fig. 1 Creep fatigue Interaction Diagram according to RCC-MRx and ASME.
Concerning the assessment of the creep-fatigue the holding periods on the fatigue life in order to interaction damage, several researchers have validate the creep-fatigue interaction diagram adopted previously proposed different approaches based on in RCC-MRx code for the P91 steel. hysteresis energy [6-9]. Takahashi et al.  evaluated 2. Material and Experimental Procedures creep damage on the basis of inelastic strain-energy density rate and creep-fatigue life using the linear sum The experimental set-up used to performr LCF (low of fatigue damage and creep damage. Other works cycle fatigue), CF (creep fatigue) and RF (relaxation propose innovative methods to evaluate creep-fatigue fatigue) tests consists of the following components: life on the basis of fracture energy [10-12] considering hydraulic press (100 kN), load cell (operation range: ± as time dependent the change in fracture energy. 100 kN), extensometer (12 mm gauged length) and Kimura et al.  have proposed a method for induction furnace (6 kW). An extensive optimization predicting creep life called the “region splitting process has been carried out on the induction furnace analysis method”. In this method, creep rupture data shape in order to keep the temperature profile constant are divided into high-stress and low-stress regions along the gauged length, achieving a tolerance within with a boundary condition of one half of the 0.2% ±2 °C. A Control Unit with embedded software allows offset yield stress. The region splitting analysis great flexibility in mixing fatigue cycling with creep method for creep rupture curves has been taken into hold times. account in the 2012 JSME code. The samples for the tests were manufactured The activity reported in this paper was planned to according to ASTM 2714-099  and have undergone perform tests on 9Cr-1Mo ferritic/martensitic steel statistic quality controls after production in order to (P91) at 550 °C combining fatigue cycles and constant verify their fulfilment to specifications in terms of tensile holding periods (in both creep-fatigue and surface roughness and dimensional tolerances. The relaxation-fatigue mode). The final aim of the activity specimens have been obtained from the 12 mm thick is to investigate how much detrimental is the effect of 9Cr1MoVNb plate manufactured by Industeel. The
20 Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91 chemical composition of the material is reported in during the hold-time. The load, on the other hand, is Table 1. The plate has undergone the following the feedback signal in tensile and compressive peaks thermal treatments: austenitization (1,060 °C—4 h), and becomes the controlled parameter during the water quenching, tempering (760 °C—3 h 20 min) and hold-time (Fig. 2). air cooling. Different from CF tests, in RF tests, the strain CF (creep fatigue) and RF (relaxation fatigue) tests remains the controlled parameter for the whole differ from standard LCF tests by the interposition of duration of the cycle, both in tensile and compressive hold-times within the cyclic testing. During CF tests, peaks and during the hold-time. The load, on the other the stress level is held constant during holding periods. hand, remains the feedback signal both in tensile and The strain is the controlled parameter in tensile and compressive peaks and during the hold-time (Fig. 3). compressive peaks and it becomes the feedback signal In all of the cases, the fatigue strain was controlled
Table 1 Nominal chemical composition of P91 steel supplied by Industeel (wt%). C Si Mn P Cr Mo Ni Al Cu Nb Ti V N Fe 0.102 0.22 0.38 0.021 8.99 0.89 0.11 0.015 0.06 0.06 0.003 0.21 0.044 Bal.
Fig. 2 CF cycle; HT tension 12 s; stress-strain behaviour.
Fig. 3 RF cycle; HT tension 600 s; stress-strain behaviour at the beginning (left), and end of HT (right).
Low Cycle Fatigue, Creep-Fatigue and Relaxation-Fatigue Tests on P91 21
in terms of total strain (elastic + plastic), which was Besides the LCF (low cycle fatigue), the CF (creep measured and controlled by the extensometer. The fatigue) and the RF (relaxation fatigue) tests, a series wave shape was triangular and the parameters of the of creep rupture tests has been performed, in test (total strain range, strain rate and frequency) are agreement with ASTM E139-11 standards . The listed below: tests have been carried out using single lever MAYES
tot =1%, 0.6% machines with auto-levelling arm device. A three